#------------------------------------------------------------------------------
#$Date: 2019-11-25 01:16:58 +0200 (Mon, 25 Nov 2019) $
#$Revision: 239846 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/35/03/4350340.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4350340
loop_
_publ_author_name
'Yamase, Toshihiro'
'Fukaya, Keisuke'
'Nojiri, Hiroyuki'
'Ohshima, Yuhgo'
_publ_section_title
;
 Ferromagnetic exchange interactions for Cu6(12+) and Mn6(12+) hexagons
 sandwiched by two B-alpha-[XW9O33]9- (X = As(III) and Sb(III)) ligands in
 D3d-symmetric polyoxotungstates.
;
_journal_issue                   19
_journal_name_full               'Inorganic chemistry'
_journal_page_first              7698
_journal_page_last               7704
_journal_paper_doi               10.1021/ic060666f
_journal_volume                  45
_journal_year                    2006
_chemical_formula_moiety         'C48 H156 As2 Cl6 Cu6 N12 O72 W18 '
_chemical_formula_sum            'C48 H156 As2 Cl6 Cu6 N12 O72 W18'
_chemical_formula_weight         6106.93
_space_group_IT_number           148
_space_group_name_Hall           '-R 3'
_space_group_name_H-M_alt        'R -3 :H'
_symmetry_cell_setting           trigonal
_symmetry_Int_Tables_number      148
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   20.33(1)
_cell_length_b                   20.33(1)
_cell_length_c                   26.35(2)
_cell_measurement_reflns_used    35919
_cell_measurement_temperature    173.1
_cell_measurement_theta_max      30.0
_cell_measurement_theta_min      3.1
_cell_volume                     9432(10)
_computing_cell_refinement       PROCESS-AUTO
_computing_data_collection       PROCESS-AUTO
_computing_data_reduction        CrystalStructure
_computing_publication_material  'CrystalStructure Ver. 3.5.1'
_computing_structure_refinement  CRYSTALS
_computing_structure_solution    SHELXS97
_diffrn_detector_area_resol_mean 10.00
_diffrn_measured_fraction_theta_full 0.9987
_diffrn_measured_fraction_theta_max 0.9987
_diffrn_measurement_device_type  'Rigaku RAXIS-RAPID'
_diffrn_measurement_method       ω
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.7107
_diffrn_reflns_av_R_equivalents  0.054
_diffrn_reflns_limit_h_max       26
_diffrn_reflns_limit_h_min       -26
_diffrn_reflns_limit_k_max       26
_diffrn_reflns_limit_k_min       -26
_diffrn_reflns_limit_l_max       34
_diffrn_reflns_limit_l_min       -34
_diffrn_reflns_number            31078
_diffrn_reflns_theta_full        27.47
_diffrn_reflns_theta_max         27.47
_exptl_absorpt_coefficient_mu    18.137
_exptl_absorpt_correction_T_max  0.015
_exptl_absorpt_correction_T_min  0.004
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details
;
    Higashi, T. (1999). Program for Absorption Correction.
    Rigaku Corporation, Tokyo, Japan.
;
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    3.225
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             8334.00
_exptl_crystal_size_max          0.40
_exptl_crystal_size_mid          0.38
_exptl_crystal_size_min          0.23
_refine_diff_density_max         1.22
_refine_diff_density_min         -2.32
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.012
_refine_ls_number_parameters     245
_refine_ls_number_reflns         4313
_refine_ls_R_factor_gt           0.0260
_refine_ls_shift/su_max          0.0000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w = 1/[0.0001Fo² + 1.0000σ(Fo²)]/(4Fo²)'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_ref         0.0830
_reflns_number_gt                4307
_reflns_number_total             4796
_reflns_threshold_expression     F²>2.0σ(F²)
_cod_data_source_file            ic060666fsi20060419_083130.cif
_cod_data_source_block           '_(nBuNH3)12[(CuCl)6(AsW9O33)2]6H2O'
_cod_original_cell_volume        9431(9)
_cod_original_sg_symbol_Hall     '- R 3'
_cod_original_sg_symbol_H-M      'R -3       '
_cod_original_formula_sum        'C48 H156 As2 Cl6 Cu6 N12 O72 W18 '
_cod_database_code               4350340
loop_
_symmetry_equiv_pos_as_xyz
x,y,z
-x,-y,-z
x+1/3,y+2/3,z+2/3
-x+1/3,-y+2/3,-z+2/3
x+2/3,y+1/3,z+1/3
-x+2/3,-y+1/3,-z+1/3
-y,x-y,z
y,-x+y,-z
-y+1/3,x-y+2/3,z+2/3
y+1/3,-x+y+2/3,-z+2/3
-y+2/3,x-y+1/3,z+1/3
y+2/3,-x+y+1/3,-z+1/3
-x+y,-x,z
x-y,x,-z
-x+y+1/3,-x+2/3,z+2/3
x-y+1/3,x+2/3,-z+2/3
-x+y+2/3,-x+1/3,z+1/3
x-y+2/3,x+1/3,-z+1/3
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
W(1) W 0.44531(2) 0.68316(2) 0.44601(1) 0.01417(9) Uani 1.00 1 d .
W(2) W 0.53542(2) 0.77781(2) 0.55254(1) 0.01237(8) Uani 1.00 1 d .
W(3) W 0.45297(2) 0.58951(2) 0.55048(1) 0.01212(8) Uani 1.00 1 d .
As(1) As 0.3333 0.6667 0.56652(5) 0.0105(2) Uani 1.00 1 d .
Cu(1) Cu 0.48503(5) 0.68536(5) 0.66752(3) 0.0129(2) Uani 1.00 1 d .
Cl(1) Cl 0.6139(1) 0.7022(1) 0.68072(8) 0.0243(5) Uani 1.00 1 d .
O(1) O 0.4834(3) 0.6886(3) 0.3871(2) 0.021(2) Uani 1.00 1 d .
O(2) O 0.6272(3) 0.8509(3) 0.5587(2) 0.022(2) Uani 1.00 1 d .
O(3) O 0.4955(3) 0.5349(3) 0.5547(2) 0.019(2) Uani 1.00 1 d .
O(4) O 0.4023(3) 0.7456(3) 0.4382(2) 0.016(1) Uani 1.00 1 d .
O(5) O 0.5307(3) 0.7650(3) 0.4785(2) 0.016(1) Uani 1.00 1 d .
O(6) O 0.4704(3) 0.6121(3) 0.4776(2) 0.020(2) Uani 1.00 1 d .
O(7) O 0.5443(3) 0.6913(3) 0.5573(2) 0.013(1) Uani 1.00 1 d .
O(8) O 0.3523(3) 0.5149(3) 0.5400(2) 0.016(1) Uani 1.00 1 d .
O(9) O 0.4132(3) 0.6754(3) 0.5324(2) 0.014(1) Uani 1.00 1 d .
O(10) O 0.4965(3) 0.7635(3) 0.6183(2) 0.015(1) Uani 1.00 1 d .
O(11) O 0.4334(3) 0.6020(3) 0.6179(2) 0.013(1) Uani 1.00 1 d .
O(12) O 0.6419(4) 0.5521(5) 0.5575(3) 0.052(3) Uani 1.00 1 d .
N(1) N 0.6229(4) 0.6276(4) 0.4672(3) 0.032(2) Uani 1.00 1 d .
N(2) N 0.5509(4) 0.5289(4) 0.6532(3) 0.030(2) Uani 1.00 1 d .
C(1) C 0.6785(6) 0.7093(6) 0.4753(4) 0.038(3) Uani 1.00 1 d .
C(2) C 0.6722(7) 0.7561(6) 0.4282(4) 0.050(3) Uani 1.00 1 d .
C(3) C 0.7175(8) 0.8425(7) 0.4377(5) 0.063(4) Uani 1.00 1 d .
C(4) C 0.7096(8) 0.8915(9) 0.3930(5) 0.081(6) Uani 1.00 1 d .
C(5) C 0.594(2) 0.490(2) 0.665(1) 0.060(7) Uiso 0.50 1 d P
C(6) C 0.574(2) 0.452(2) 0.717(1) 0.080(9) Uiso 0.50 1 d P
C(7) C 0.619(2) 0.410(1) 0.7210(7) 0.17(1) Uani 1.00 1 d .
C(8) C 0.580(1) 0.389(1) 0.7771(8) 0.16(1) Uani 1.00 1 d .
C(9) C 0.550(1) 0.463(1) 0.6811(8) 0.033(4) Uiso 0.50 1 d P
C(10) C 0.630(1) 0.481(1) 0.6920(9) 0.046(6) Uiso 0.50 1 d P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.003 0.002
;
International Tables for Crystallography
(1992, Vol. C, Tables 4.2.6.8 and 6.1.1.4)
;
N N 0.006 0.003
;
International Tables for Crystallography
(1992, Vol. C, Tables 4.2.6.8 and 6.1.1.4)
;
Cu Cu 0.320 1.265
;
International Tables for Crystallography
(1992, Vol. C, Tables 4.2.6.8 and 6.1.1.4)
;
Cl Cl 0.148 0.159
;
International Tables for Crystallography
(1992, Vol. C, Tables 4.2.6.8 and 6.1.1.4)
;
As As 0.050 2.006
;
International Tables for Crystallography
(1992, Vol. C, Tables 4.2.6.8 and 6.1.1.4)
;
W W -0.849 6.872
;
International Tables for Crystallography
(1992, Vol. C, Tables 4.2.6.8 and 6.1.1.4)
;
O O 0.011 0.006
;
International Tables for Crystallography
(1992, Vol. C, Tables 4.2.6.8 and 6.1.1.4)
;
H H 0.000 0.000
;
International Tables for Crystallography
(1992, Vol. C, Table 6.1.1.4)
;
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_publ_flag
O(1) W(1) O(4) 101.8(3) yes
O(1) W(1) O(5) 99.6(2) yes
O(1) W(1) O(6) 99.1(3) yes
O(1) W(1) O(9) 169.4(3) yes
O(4) W(1) O(5) 89.3(3) yes
O(4) W(1) O(6) 159.0(2) yes
O(4) W(1) O(9) 86.8(2) yes
O(5) W(1) O(6) 89.6(2) yes
O(5) W(1) O(9) 74.0(2) yes
O(6) W(1) O(9) 72.7(2) yes
O(2) W(2) O(5) 99.7(2) yes
O(2) W(2) O(7) 103.6(3) yes
O(2) W(2) O(9) 172.1(2) yes
O(2) W(2) O(10) 103.9(2) yes
O(5) W(2) O(7) 87.9(3) yes
O(5) W(2) O(9) 72.6(2) yes
O(5) W(2) O(10) 155.9(2) yes
O(7) W(2) O(9) 74.9(2) yes
O(7) W(2) O(10) 91.4(3) yes
O(9) W(2) O(10) 83.9(2) yes
O(3) W(3) O(6) 97.1(3) yes
O(3) W(3) O(7) 99.1(2) yes
O(3) W(3) O(8) 100.8(3) yes
O(3) W(3) O(9) 168.7(2) yes
O(3) W(3) O(11) 103.7(3) yes
O(6) W(3) O(7) 83.1(2) yes
O(6) W(3) O(9) 73.3(3) yes
O(6) W(3) O(11) 157.6(3) yes
O(7) W(3) O(9) 74.3(2) yes
O(7) W(3) O(11) 85.6(2) yes
O(9) W(3) O(11) 85.0(2) yes
Cl(1) Cu(1) O(10) 106.8(2) yes
Cl(1) Cu(1) O(11) 106.4(2) yes
O(10) Cu(1) O(11) 93.0(2) yes
W(1) O(5) W(2) 121.7(2) yes
W(1) O(6) W(3) 120.5(4) yes
W(2) O(7) W(3) 119.9(3) yes
W(1) O(9) W(2) 91.3(2) yes
W(1) O(9) W(3) 93.4(2) yes
W(1) O(9) As(1) 134.6(3) yes
W(2) O(9) W(3) 90.5(2) yes
W(2) O(9) As(1) 118.5(3) yes
W(3) O(9) As(1) 117.8(2) yes
W(2) O(10) Cu(1) 127.3(4) yes
W(3) O(11) Cu(1) 133.6(2) yes
C(2) C(1) N(1) 108.0(8) yes
C(3) C(2) C(1) 111.8(9) yes
C(4) C(3) C(2) 113(1) yes
C(6) C(5) N(2) 111(2) yes
C(9) C(5) C(10) 96(3) yes
C(7) C(6) C(5) 104(2) yes
C(8) C(7) C(10) 121(2) yes
C(8) C(7) C(6) 82(2) yes
C(10) C(9) N(2) 110(1) yes
C(7) C(10) C(9) 103(1) yes
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_publ_flag
W(1) O(1) 1.713(5) yes
W(1) O(4) 1.879(8) yes
W(1) O(5) 1.905(4) yes
W(1) O(6) 1.944(7) yes
W(1) O(9) 2.353(5) yes
W(2) O(2) 1.716(5) yes
W(2) O(5) 1.963(5) yes
W(2) O(7) 1.860(7) yes
W(2) O(9) 2.370(4) yes
W(2) O(10) 1.866(5) yes
W(3) O(3) 1.718(8) yes
W(3) O(6) 1.966(5) yes
W(3) O(7) 1.979(4) yes
W(3) O(8) 1.860(4) yes
W(3) O(9) 2.311(7) yes
W(3) O(11) 1.866(5) yes
As(1) O(9) 1.784(6) yes
Cu(1) Cl(1) 2.490(3) yes
Cu(1) O(10) 1.972(6) yes
Cu(1) O(11) 1.976(5) yes
N(1) C(1) 1.48(1) yes
N(2) C(5) 1.48(4) yes
N(2) C(9) 1.53(3) yes
C(1) C(2) 1.61(2) yes
C(2) C(3) 1.54(2) yes
C(3) C(4) 1.60(2) yes
C(5) C(6) 1.54(4) yes
C(6) C(7) 1.53(6) yes
C(7) C(8) 1.63(3) yes
C(7) C(10) 1.54(4) yes
C(9) C(10) 1.51(4) yes
